If you can't read please download the document

View

216Download

0

Tags:

Embed Size (px)

DESCRIPTION

simulation

13th International LS-DYNA Users Conference Session: Simulation

1-1

Benchmark of Frequency Domain Methods for Composite Materials with Damage using LS-DYNA

Myeong-Gyu Bae*, Seonwoo Lee

THEME Engineering, Inc.

Abstract The composite material is widely used in the structures as aircrafts, satellites, ships,

automobiles, and so on which demand light weight and high performance. A various type of damage could occur through low-speed impacts and fatigue loads. It is generally known that the assessment of the natural frequency by vibration testing is a very attractive method as a Non-Destructive Test (NDT) and the vibration response of a composite structure can be utilized as an indicator of damage. In this paper, a desirable FE modeling technique regarding composite types

(Laminated/Sandwich) and laminate methods of composite material were investigated using LS-DYNA. Firstly, according to the laminated properties of composite material (number of layers,

anisotropy, shape, etc.), frequency responses were compared between the latest theories and the latest version of LS-DYNA. Secondly, various types of damage in cantilever beam with composite material were represented and estimated in FE model and those frequency responses were compared among experiments, LS-DYNA, and other FE code. Finally, delamination phenomenon in rectangular plate with composite material was represented and estimated in FE model and those frequency responses were compared between experiment and LS-DYNA.

It was evaluated and verified that the prediction for the tendency of natural frequency using the frequency domain method in LS-DYNA could be appropriate for composite materials with or without damage.

1. Introduction The applications of composite materials have become common in various fields of industries.

These materials have higher stiffness and strength to weight ratio and also offer many advantages in the designing and manufacturing of structures. The application of woven fabric composites in engineering structures has been significantly

increased due to attractive characteristics such as flexible processing options, low fabrication cost while also possessing adequate mechanical properties. The laminated composite plates are basic structural components used in a variety of engineering

structures. Composite plate structures often operate in complex environmental conditions and are frequently exposed to a variety of dynamic excitations. A measurement of the natural frequency by vibration testing is a very attractive method as Non-Destructive Test (NDT). The vibration test would not require access to the whole surface and the time taken to perform the test can be very small. Thus the vibration response of a composite plate can be utilized as an indicator of damage estimation.

This paper deals with the evaluation and verification on the frequency responses of composite structure with damage and those results by modal and frequency domain analysis using the latest version of LS-DYNA are compared among the latest theories, experiment, and other FE code.

Session: Simulation 13th International LS-DYNA Users Conference

1-2

2. Analysis solutions of theories and responses of LS-DYNA 2.1 Theories The Classical Laminate Plate Theory (CLPT) which ignores the effect of transverse shear

deformation becomes inadequate for the analysis of multilayer composites. In general the CLPT often underpredicts deflections and overpredicts natural frequencies and bucking loads. And the first-order theories (FSDTs) assume linear in-plane stresses and displacements respectively through the laminate thickness. Since the FSDT accounts for layerwise constant states of transverse shear stress, shear correction coefficients are needed to rectify the unrealistic variation of the shear strain/stress through the thickness and which ultimately define the shear strain energy. In order to overcome the limitations of FSDT, higher-order shear deformation theories (HSDTs) have been developed through many other previous studies [1, 2, 3, 4, 5]. In displacement model, in order to approximate the three-dimensional elasticity problem to a

two-dimensional plate problem, the displacement components (, y, z, t), (, y, z, t) and (, y, z, t) at any point in the plate space is expanded in a Taylors series in terms of the thickness coordinate. The displacement field which satisfies the above criteria may be assumed in the following form: Model (1) Kant-Manjunatha (, y, z, t) = (, , ) + (, , ) + (, , ) +(, , ), (, y, z, t) = (, , ) + (, , ) + (, , ) +(, , ), (, y, z, t) = (, , ) + (, , ) + (, , ) +(, , ). (1)

Further if the variation of transverse displacement component (, y, z) in Eq. (1) is assumed

constant through the plate thickness and thus setting = 0. Then the displacement field may be expressed as: Model (2) Pandya Kant (, y, z) = (, ) + (, ) + (, ) +(, ), (, y, z) = (, ) + (, ) + (, ) +(, ), (, y, z) = (, ). (2) The parameters , , , , , and in Eq. (1) and Eq. (2) are the higher-order terms in

the Taylors series expansion and they represent higher-order transverse cross-sectional deformation modes. In addition to the above, the displacement models of other theories as present in table.1 are as blow: Model (3) Reddy

(, y, z) = (, ) + (, ) 43

(, ) +

,

(, y, z) = (, ) + (, ) 43

(, ) +

y ,

(, y, z) = (, ). (3)

13th International LS-DYNA Users Conference Session: Simulation

1-3

Model (4) Senthilnathan et al.

(, y, z) = (, )

43

,

(, y, z) = (, ) y

43

y ,

(, y, z) = (, ) + (, ). (4) Model (5) Whitney-Pagano (, y, z) = (, ) + (, ), (, y, z) = (, ) + (, ), (, y, z) = (, ). (5) Table.1 Displacement models (shear deformation theories) compared Source (Eq.) Theory Year [Ref.] Degrees of freedom Transverse normal Model (1) HSDT 1988 [2] 12 Considered Model (2) HSDT 1988 [3] 9 Not considered Reddy(3) HSDT 1984 [4] 5 Not considered Senthilnathan et al.(4) HSDT 1987 [5] 4 Not considered Whitney-Pagano(5) FSDT 1970 [6] 5 Not considered

Fig.1 Laminate geometry with positive set of lamina/laminate reference axes, displacement components and fiber orientation

The geometry of a two-dimensional laminated composite plate with positive set of coordinate

axes and the physical middle plane displacement terms which used in above theories are shown in Fig. 1. Assuming that the cross-ply rectangular plate is simply supported in such a manner that normal displacement is admissible, but the tangential displacement is not, the following boundary conditions are appropriate:

TYPICAL LAMINA

1 2

3, z

(1,2,3) LAMINA REFERENCE AXES

z, 3

w0

v0

y

a

b u0 x

L = 1L = 2

zL zL+1

L = NL

( x,y,z ) LAMINATE REFERENCE AXES

LAMINATE MID-PLANE

Session: Simulation 13th International LS-DYNA Users Conference

1-4

At edges = 0and = : = 0; = 0; = 0; = 0; = 0; = 0; = 0; = 0; = 0;M = 0; = 0;N = 0.

At edges = 0and = : = 0; = 0; = 0; = 0; = 0; = 0; = 0; = 0; = 0;M = 0; = 0;N = 0.

2.2 FE Model in LS-DYNA

Finite element analyses using LS-DYNA were carried out to evaluate the frequency response of various types of composite material models made of laminated types and composite types. All these composite plates with simply supported boundary conditions as stated above were modeled with 4-node quadrilateral shell elements and 1 mm mesh size regardless of specimen size. And *PART_COMPOSITE card was used for the method of stacking of composite layers and *MAT_COMPOSITE_DAMAGE (*MAT_022) was applied as a representative constitutive model for the orthotropic characteristics of material properties.

Fig.2 Composite material types (Left) and boundary condition (right) of FE model in LS-DYNA 2.3 Numerical results and discussion The nondimensionalized natural frequency of general rectangular composite and sandwich plates with simple support are considered for comparison. The nondimensinalized natural frequencies computed using various models for 2, 4, 6 and 10 layer antisymmetric cross-ply laminate with layers of equal thickness are given in Table.2. The orthotropic material properties of individual layers in all the above laminates considered are = open, = , = = 0.6, = 0.5, = = = 0.25.

Three-dimensional elasticity solution and other 5 theories (4 HSDTs and 1 FSFT) are considered for comparison with LS-DYNA as in Table 2. It shows that a very similar tendency of frequency responses are comparable between LS-DYNA and all five theories. For all the laminated types considered, at lower range of ratio equal to 3 and 10 the error in LS-DYNA is relatively less. Whereas for 2, 4, 6 layer laminates at higher range of ratio equal to 20-40 the error in LS-DYNA and FSDT (Whitney-Pagano's theory) increases.

The variation of natural frequencies with respect to side-to-thickness ratio is presented in Table 3. It shows that a very similar results of frequency responses are also comparable between LS-DYNA and all five theories according to thickness changes. Consequently, in laminated compos